Pré-visualização3 páginas

D3, Q1, 20\u3bcm, 500kg/m3) b) TI (Q1, 20\u3bcm, 500kg/m3) Figure 8: Trajectories of particles in tundishes The injection of a particle is set. The original injection position is on the inlet surface. The injected particles are set with different diameters and densities. 2,000 particles are released each time and their trajectories are calculated out with discrete random walk model. Each injection condition is repeated five times and then the total separation ratios are calculated. Twenty representative trajectories of inclusion particles in SFT and a tundish with TI are shown in Fig. 8. It can be seen that the trajectories for the same kind of inclusion particle are different. In the tundish with SC, most particles have longer trajectories in the impact zone than those in the tundish with TI. This can enhance the removal of inclusion to slag-steel interface. Moreover, in the zone above the outlet, it can be seen that inclusion particles in the tundish with TI have greater possibility to go into mold than those in the tundish with SC. Comparison of removal possibility The influence of density on separation ratio is given in Fig. 9. It can be seen that the differences of density have a minor influence on separation ratio within the density range of 400~600kg/m3. Moreover, according to the weight of inclusion distribution (shown in Fig. 10) from experimental samples, particles that are larger than 75\u3bcm have little significance and can be neglected during simulation process. Figure 9: Relationships of removal ratio and density of inclusion particles For larger diameters of particle (50\u3bcm), the separation ratio of tundish with TI is higher than that of SFT. The reason for this is the short distance between the dam and the first weir or between dam and SC which can be seen from the trajectories shown in Fig. 11 (a, b). Because of these narrow spaces, the upward flow is very quick and it can be reflected instantly downward. Consequently, the entrainment possibility of inclusion particles to slag-steel interface is decreased for inclusion particles. The SFT has been revised to alleviate this phenomenon. Both of the distances between the dam and the first weir and between the weir and SC have been extended 100mm in one simulation. It can be seen from Fig. 11 (c) that the strong upward flow is weakened. As a result, the separation ratios of inclusions are improved as shown in Table 3, particularly for the 20\u3bcm diameter particles. Figure 10: The size distribution of inclusion in weight extracted from steel by Slimes method (Zhang, et al., 2000) Diameter, \u3bcm Tundish 20 50 60 80 TI, % 82.00 94.95 97.27 99.10 SFT, % 86.40 92.30 94.09 97.67 Adjusted SFT, % 89.85 93.68 95.19 97.95 Table 3: Separation ratio in different kinds of tundish (\u3c1=500kg/m3) Fifth International Conference on CFD n the Process Industries CSIRO, Melbourne, Australia 13-15 December 2006 a) SFT b) TI c) Adjusted SFT Figure 11: Trajectories of particles It should be pointed out here that the original positions of flow control devices were optimized for tundish with TI. However, the results show that they are no more suitable for SFT. For different design of flow control schemes, their positions should be relocated for optimum operation. CONCLUSIONS A new swirling flow tundish has been developed and modelled by physical and mathematical methods. The numerical model is validated by measured RTD curves and flow field respectively. The flow field, the movement and separation of inclusions are examined too. The conclusion can be drawn as follows. 1. Small inclusions have higher probability of flotation to slag-steel interface in SFT than the tundish with TI. The separation ratios show that SFT has a greater ability to remove small inclusion (such as 20\u3bcm) than the tundish with TI. 2. For different designs of tundish, the positions of all flow control devices should be relocated for optimum metallurgical effects. ACKNOWLEDGEMENT Q. F. HOU\u2019s grateful acknowledgement is made to the Centre for Simulation and Modelling of Particulate Systems for the visiting fellowship. REFERENCES D. Mazumdar and R. I. L. Guthrie, (1999), Physical and mathematical modelling of continuous casting tundish systems, ISIJ Int., 39, 524. J. d. J. Barreto-Sandoval, A. W. D. Hills, M. A. Barron-Meza and R. D. Morales, (1996), Physical modelling of tundish plasma heating and its mathematical interpretation, ISIJ Int., 36, 1174. A. Ramos-Banderas, R. D. Morales, L. Garcia-Demedices and M. Diaz-Cruz, (2003), Mathematical simulation and modeling of steel flow with gas bubbling in trough type tundishes, ISIJ Int., 43, 653. Y. Miki, S. Ogura and T. Fujii, (1996), Separation of inclusions from molten steel in a tundish by use of a rotating electromagnetic field, Kawasaki Steel Technical Report, 67. Z. Zou, Q. Hou, S. Kuang, et al.: "Feasibility Study of a Swirling Flow Tundish", 2nd international conference on process development in iron and steelmaking, Luleå Sweden, 2004. Q. F. Hou and Z. S. Zou, (2005a), Study on fluid flow in swirling chamber of swirling flow tundish, Kang T'ieh/Iron and Steel (Peking), 40, 33. Q. Hou and Z. Zou, (2005b), Numerical and physical simulation of flow patterns in a swirling flow tundish, Steel Res. Int., 76, 726. V. Chevrier and A. W. Cramb, (2005), Observation and measurement of bubble separation at liquid steel-slag interfaces, Scand. J. Metall., 34, 89. K. Beskow, J. Jia, C. H. P. Lupis and S. C. Du, (2002), Chemical characteristics of inclusions formed at various stages during the ladle treatment of steel, Ironmaking & Steelmaking, 29, 427. A. Haider and O. Levenspiel, (1989), Drag coefficient and terminal velocity of spherical and nonspherical particles, Powder Technology, 58, 63. A. K. Sinha and Y. Sahai, (1993), Mathematical modeling of inclusion transport and removal in continuous casting tundishes, ISIJ Int., 33, 556. S. Lopez-Ramirez, J. D. J. Barreto, J. Palafox-Ramos, R. D. Morales and D. Zacharias, (2001), Modeling study of the influence of turbulence inhibitors on the molten steel flow, tracer dispersion, and inclusion trajectories in tundishes, Metallurgical and Materials Transactions B: Process Metallurgy and Materials Processing Science, 32, 615. L. F. Zhang, S. Taniguchi and K. K. Cai, (2000), Fluid flow and inclusion removal in continuous casting tundish, Metall. Mater. Trans. B-Proc. Metall. Mater. Proc. Sci., 31, 253. D. Bouris and G. Bergeles, (1998), Investigation of inclusion re-entrainment from the steel-slag interface, Metallurgical and Materials Transactions B: Process Metallurgy and Materials Processing Science, 29, 641. Y. He and Y. Sahai, (1987), The Effect of Tundish Wall Inclination on the Fluid-Flow and Mixing - a Modeling Study, Metallurgical Transactions B-Process Metallurgy, 18, 81. B. E. Launder and D. B. Spalding, (1974), The numerical computation of turbulent flows, Computer Methods in Applied Mechanics and Engineering, 3, 269. A. Kumar, S. C. Koria and D. Mazumdar, (2004), An assessment of fluid flow modelling and residence time distribution phenomena in steelmaking tundish systems, ISIJ Int., 44, 1334. Y. Sahai and T. Emi, (1996), Criteria for water modeling of melt flow and inclusion removal in continuous casting tundishes, ISIJ Int., 36, 1166. 1 School of Materials and Metallurgy, Northeastern University, Shenyang, 110004, China 2 Centre for Simulation and Modelling of Particulate Systems, School of Materials Science and Engineering, University of New South Wales, Sydney, NSW 2052, Australia REFERENCES